High-temperature components in thermal power plants are subjected to creep-fatigue loading where creep cavities initiate and grow on grain boundaries. Development of life assessment methods of high-temperature components in gas turbine for maintenance and operating cost reduction is strongly demanded by Japanese utilities. Especially, first row blades are subjected to complicated thermomechanical-fatigue (TMF) loading during start, steady state, stop cycles. Therefore it is important to clarify the TMF life property of blade materials to develop a life assessment procedure. In this study, tension-torsion biaxial TMF tests have been performed between $450°C$ and $870°C$ on a Ni-base directional solidified superalloy. Strain ratio $ϕ$ was defined as shear strain range, $Δγ$, to normal strain range, $Δε$, and $ϕ$ varied from 0 to infinity. The “Blade wave form,” which simulated temperature and strain condition of the blade surface, was employed. The biaxial TMF tests were also carried out on coated specimens with CoCrAlY. Fatigue life under the biaxial TMF loading showed strain ratio dependency giving shorter life with increasing $ϕ$. Considering biaxial stress effect on the failure life, an equivalent shear strain range was derived based on the $Γ$-plane theory, and the biaxial TMF life was well correlated with the equivalent shear strain range. The biaxial TMF life was reduced by introducing strain hold duration at the maximum temperature. The maximum stress increased by introducing the hold time due to increasing mean stress level in the Blade wave form. It was concluded that creep damage gradually accumulated during cycles resulting in reduction in the TMF life. The nonlinear creep-fatigue damage accumulation model was applied to predict failure life of the hold time tests. As a result, the failure lives were predicted within a factor of 1.5 on the observed life. It was found that the fatigue life of CoCrAlY coated material reduced $1∕2$ to $1∕3$ from that of the substrate. From observation of the longitudinal section of the coated specimens, many cracks started from the coating surface and penetrated into the substrate. It was concluded that the CoCrAlY coating reduced the biaxial TMF life due to acceleration of crack initiation period in the substrate.

1.
Ogata
,
T.
, and
Yamamoto
,
M.
, 2001, “
Life Evaluation of IN738LC Under Biaxial Thermo-Mechanical Fatigue
,”
Proceedings of 6th International Conference on Biaxial and Multiaxial Fatigue and Fracture
,
M.
de Freitas
, ed.,
ESIS
,
Lisbon
, pp.
839
848
.
2.
Ogata
,
T.
,
Sakai
,
T.
,
Yaguchi
,
M.
,
Fukutomi
,
H.
, and
Takahashi
,
T.
, 2002, “
Analytical and Nondestructive Damage Assessment of Gas Turbine Blade
,”
Proceedings of International Conference on “Advances in Life Assessment and Optimization of Fossil Power Plants
,”
EPRI
,
Florida
.
3.
Ogata
,
T.
, and
Nomoto
,
A.
, 2002, “
Effect of CoCrAlY Coating on Thermo-Mechanical Fatigue of Inconel 738LC
,”
Proceedings of International Conference on Fatigue 2002
,
EMAS
,
Stockholm
.
4.
Hales
,
R.
, 1980, “
A Quantitative Metallographic Assessment of Structural Degradation of Type 316 Stainless Steel During Creep-Fatigue
,”
Fatigue Fract. Eng. Mater. Struct.
,
3
, pp.
339
356
.
5.
Ogata
,
T.
, and
Arai
,
M.
, 1998, “
Continuous Observations of Creep-Fatigue Damage Process
,”
Fatigue Fract. Eng. Mater. Struct.
8756-758X,
21
, pp.
873
884
.
6.
Imamura
,
K.
,
Ogata
,
T.
, and
Yamamoto
,
M.
, 2002, “
Evaluation of High Temperature Strength Properties of a Long-Term Service Exposed Rotor
,”
Proceedings of International Conference on “Advanced in Life Assessment and Optimization of Fossil Power Plants
,”
EPRI
,
Florida
.
7.
Yamamoto
,
M.
,
Yaguchi
,
M.
, and
Ogata
,
T.
, 2000, “
Development of High Temperature Strength Evaluation Method for Nickel-Based Directionally Solidified Superalloy
,” Denchuken Report No. T99024, in Japanese.
8.
Viswanathan
,
R.
,
Schiebel
,
J.
, and
Gandy
,
D. W.
, 2000, “
Life Management System for Combustion Turbine Blades and Vanes,” “Life Assessment of Hot Section Gas Turbine Components
,” IOM Communications, pp.
249
269
.
9.
Brown
,
M. W.
, and
Miller
,
K. J.
, 1973, “
A Theory for Fatigue Failure Under Multiaxial Stress-Strain Conditions
,”
Proc. Inst. Mech. Eng.
0020-3483,
187
, pp.
745
755
.
10.
Nitta
,
A.
,
Ogata
,
T.
, and
Kuwabara
,
K.
, 1989, “
Fracture Mechanism and Life Assessment Under High-Strain Biaxial Cyclic Loading of Type 304 Stainless Steel
,”
Fatigue Fract. Eng. Mater. Struct.
8756-758X,
12
, pp.
77
92
.
11.
Ogata
,
T.
, and
Nitta
,
A.
, 1994, “
Creep-Fatigue Damage Assessment Model for Boiler and Turbine Materials in Fossil Power Plant
,” ASME PVP-Vol. 276, pp.
97
105
.